Magnetocaloric Behavior in Ternary Europium Indides EuT5In: Probing the Design Capability of First-Principles-Based Methods on the Multifaceted Magnetic Materials
Bigun, Inna; Steinberg, Simon; Smetana, Volodymyr; Mudryk, Yaroslav; Kalychak, Yaroslav; Havela, Ladislav; Pecharsky, Vitalij; Mudring, Anja-Verena; Chemistry of Materials  (2017) –; doi:10.1021/acs.chemmater.6b04782

data_4002711
_publ_section_title
;
 Magnetocaloric Behavior in Ternary Europium Indides EuT5In: Probing the
 Design Capability of First-Principles-Based Methods on the Multifaceted
 Magnetic Materials
;
_journal_name_full               'Chemistry of Materials'
_journal_paper_doi               10.1021/acs.chemmater.6b04782
_journal_year                    2017
_chemical_formula_sum            'Ag5 Eu In'
_chemical_formula_weight         806.13
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   9.120(2)
_cell_length_b                   5.6453(14)
_cell_length_c                   11.437(3)
_cell_measurement_reflns_used    1773
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      31.68
_cell_measurement_theta_min      4.61
_cell_volume                     588.8(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0264
_diffrn_reflns_av_sigmaI/netI    0.0420
_diffrn_reflns_limit_h_max       3
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            1773
_diffrn_reflns_theta_full        31.68
_diffrn_reflns_theta_max         31.68
_diffrn_reflns_theta_min         4.61
_exptl_absorpt_coefficient_mu    30.452
_exptl_absorpt_correction_T_max  0.2
_exptl_absorpt_correction_T_min  0.1
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'Blessing, 1995'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    9.093
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregular fragment'
_exptl_crystal_F_000             1388
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.07
_refine_diff_density_max         2.085
_refine_diff_density_min         -1.950
_refine_diff_density_rms         0.481
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_matrix_type           full
_refine_ls_number_parameters     40
_refine_ls_number_reflns         960
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.051
_refine_ls_R_factor_all          0.0511
_refine_ls_R_factor_gt           0.0363
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0369P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0773
_refine_ls_wR_factor_ref         0.0830
_reflns_number_gt                751
_reflns_number_total             960
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm6b04782_si_003.cif
_cod_data_source_block           EuAg5In
_cod_original_cell_volume        588.9(2)
_cod_original_sg_symbol_H-M      Pnma
_cod_database_code               4002711